LMucko/crystallography-open-database huggingface dataset:
Unusual magnetic properties of the heavy-fermion compound Ce Co Ge3
Pecharskii, V.K.; Hyun, O.B.; Gschneidner, K.A.jr.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 47 (1993) 11839–11847; doi:

data_1527922
_publ_section_title
;
 Unusual magnetic properties of the heavy-fermion compound Ce Co Ge3
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              11839
_journal_page_last               11847
_journal_volume                  47
_journal_year                    1993
_chemical_formula_sum            'Ce Co Ge3'
_space_group_IT_number           107
_symmetry_space_group_name_Hall  'I 4 -2'
_symmetry_space_group_name_H-M   'I 4 m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.3192
_cell_length_b                   4.3192
_cell_length_c                   9.8298
_cell_volume                     183.380
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Pecharskii_PRBMDO_1993_270.cif
_cod_data_source_block           Ce1Co1Ge3
_cod_original_cell_volume        183.3797
_cod_original_formula_sum        'Ce1 Co1 Ge3'
_cod_database_code               1527922
Unusual magnetic properties of the heavy-fermion compound Ce Co Ge3
Pecharskii, V.K.; Hyun, O.B.; Gschneidner, K.A.jr.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 47 (1993) 11839–11847; doi:

data_1527923
_publ_section_title
;
 Unusual magnetic properties of the heavy-fermion compound Ce Co Ge3
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              11839
_journal_page_last               11847
_journal_volume                  47
_journal_year                    1993
_chemical_formula_sum            'Co Ge3 La'
_space_group_IT_number           107
_symmetry_space_group_name_Hall  'I 4 -2'
_symmetry_space_group_name_H-M   'I 4 m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.3497
_cell_length_b                   4.3497
_cell_length_c                   9.8679
_cell_volume                     186.700
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Pecharskii_PRBMDO_1993_345.cif
_cod_data_source_block           Co1Ge3La1
_cod_original_cell_volume        186.6996
_cod_original_formula_sum        'Co1 Ge3 La1'
_cod_database_code               1527923
The Crystal Structure of Ammonium Heptafluorothorate, Ammonium Catena-di-mue-fluoro-pentafluorothorate(IV)
Penneman, R.A.; Ryan, R.R.; Kressin, I.K.; Acta Crystallographica B (24,1968-38,1982) 27 (1971) 2279–2283; doi:

data_2106414
_publ_section_title
;
 The Crystal Structure of Ammonium Heptafluorothorate, Ammonium
 Catena-di-mue-fluoro-pentafluorothorate(IV)
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              2279
_journal_page_last               2283
_journal_volume                  27
_journal_year                    1971
_chemical_formula_sum            'F7 H12 N3 Th'
_chemical_name_systematic        '(N H4)3 Th F7'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.944
_cell_length_b                   7.928
_cell_length_c                   7.041
_cell_volume                     778.369
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Penneman_ACBCAR_1971_931.cif
_cod_data_source_block           H12F7N3Th1
_cod_original_cell_volume        778.3687
_cod_original_formula_sum        'H12 F7 N3 Th1'
_cod_database_code               2106414
The Crystal and Molecular Structure of Tetraphosphorus(II) Triselenodiiodide
Penney, G.J.; Sheldrick, G.M.; Acta Crystallographica B (24,1968-38,1982) 26 (1970) 2092–2095; doi:

data_2106415
_publ_section_title
;
 The Crystal and Molecular Structure of Tetraphosphorus(II)
 Triselenodiiodide
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              2092
_journal_page_last               2095
_journal_volume                  26
_journal_year                    1970
_chemical_formula_sum            'I2 P4 Se3'
_chemical_name_systematic        'P4 Se3 I2'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.78
_cell_length_b                   16.32
_cell_length_c                   6.8
_cell_volume                     1085.345
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Penney_ACBCAR_1970_1041.cif
_cod_data_source_block           I2P4Se3
_cod_database_code               2106415
Crystal and molecular structure of tetraphosphorus pentaselenide
Penney, G.J.; Sheldrick, G.M.; Journal of the Chemical Society A: Inorganic, Physical, Theoretical (1966-1971) 1971 (1971) 245–248; doi:

data_1527924
_publ_section_title
;
 Crystal and molecular structure of tetraphosphorus pentaselenide
;
_journal_name_full
;
Journal of the Chemical Society A: Inorganic, Physical, Theoretical (1966-1971)
;
_journal_page_first              245
_journal_page_last               248
_journal_volume                  1971
_journal_year                    1971
_chemical_formula_sum            'P4 Se5'
_space_group_IT_number           33
_symmetry_space_group_name_Hall  'P -2ac -2n'
_symmetry_space_group_name_H-M   'P n 21 a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   12.79
_cell_length_b                   11.19
_cell_length_c                   6.66
_cell_volume                     953.180
_citation_journal_id_ASTM        JCSIAP
_cod_data_source_file            Penney_JCSIAP_1971_1862.cif
_cod_data_source_block           P4Se5
_cod_original_cell_volume        953.1798
_cod_original_sg_symbol_Hall     'P 2c -2n (-x,z,y)'
_cod_database_code               1527924
The crystal structure of the strontium and lead tetraborates, Sr O (B2 O3)2 and Pb O (B2 O3)2
Perloff, A.; Block, S.; Acta Crystallographica (1,1948-23,1967) 20 (1966) 274–279; doi:

data_2310461
_publ_section_title
;
 The crystal structure of the strontium and lead tetraborates, Sr O (B2
 O3)2 and Pb O (B2 O3)2
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              274
_journal_page_last               279
_journal_volume                  20
_journal_year                    1966
_chemical_formula_sum            'B4 O7 Sr'
_chemical_name_systematic        'Sr B4 O7'
_space_group_IT_number           31
_symmetry_space_group_name_Hall  'P -2 2ac'
_symmetry_space_group_name_H-M   'P 21 n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.237
_cell_length_b                   4.431
_cell_length_c                   10.706
_cell_volume                     200.996
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Perloff_ACCRA9_1966_1113.cif
_cod_data_source_block           B4O7Sr1
_cod_original_sg_symbol_Hall     'P 2ac -2 (z,y,-x)'
_cod_original_formula_sum        'B4 O7 Sr1'
_cod_database_code               2310461
Structure cristalline et moleculaire du complexe tetranucleaire K2 (U O2)4 Cl4 O2 (O H)2 (H2 O)6
Perrin, A.; le Marouille, J. Y.; Acta Crystallographica B (24,1968-38,1982) 33 (1977) 2477–2481; doi:

data_2106416
_publ_section_title
;
 Structure cristalline et moleculaire du complexe tetranucleaire K2 (U
 O2)4 Cl4 O2 (O H)2 (H2 O)6
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              2477
_journal_page_last               2481
_journal_volume                  33
_journal_year                    1977
_chemical_formula_sum            'Cl4 H14 K2 O18 U4'
_chemical_name_systematic        'K2 (U O2)4 Cl4 O2 (O H)2 (H2 O)6'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                110.5
_cell_angle_beta                 96.3
_cell_angle_gamma                138.71
_cell_formula_units_Z            1
_cell_length_a                   12.15
_cell_length_b                   12.33
_cell_length_c                   8.026
_cell_volume                     592.699
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Perrin_ACBCAR_1977_587.cif
_cod_data_source_block           H14Cl4K2O18U4
_cod_original_cell_volume        592.6987
_cod_original_formula_sum        'H14 Cl4 K2 O18 U4'
_cod_database_code               2106416
The crystal structure of brewsterite, (Sr, Ba, Ca) Al2 Si6 O16 (H2 O)5
Perrotta, A.J.; Smith, J.V.; Acta Crystallographica (1,1948-23,1967) 17 (1964) 857–862; doi:

data_2310462
_publ_section_title
;
 The crystal structure of brewsterite, (Sr, Ba, Ca) Al2 Si6 O16 (H2 O)5
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              857
_journal_page_last               862
_journal_volume                  17
_journal_year                    1964
_chemical_formula_sum            'Al1.98 H9.8 O20.9 Si6.02 Sr'
_chemical_name_systematic        'Sr (Al1.98 Si6.02 O16) (H2 O)4.9'
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 94.3
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.772
_cell_length_b                   17.50999
_cell_length_c                   7.744
_cell_volume                     915.681
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Perrotta_ACCRA9_1964_1720.cif
_cod_data_source_block           H9.8Al1.98O20.9Si6.02Sr1
_cod_original_cell_volume        915.6805
_cod_original_formula_sum        'H9.8 Al1.98 O20.9 Si6.02 Sr1'
_cod_database_code               2310462
The crystal structure of Ba Al2 O4
Perrotta, A.J.; Smith, J.V.; Bulletin de la Societe Francaise de Mineralogie et de Cristallographie (72,1949-100,1977) 91 (1968) 85–87; doi:

data_1527925
_publ_section_title
;
 The crystal structure of Ba Al2 O4
;
_journal_name_full
;
Bulletin de la Societe Francaise de Mineralogie et de Cristallographie 
(72,1949-100,1977)
;
_journal_page_first              85
_journal_page_last               87
_journal_volume                  91
_journal_year                    1968
_chemical_formula_sum            'Al2 Ba O4'
_chemical_name_systematic        'Ba Al2 O4'
_space_group_IT_number           182
_symmetry_space_group_name_Hall  'P 6c 2c'
_symmetry_space_group_name_H-M   'P 63 2 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   5.218
_cell_length_b                   5.218
_cell_length_c                   8.781
_cell_volume                     207.054
_citation_journal_id_ASTM        BUFCAE
_cod_data_source_file            Perrotta_BUFCAE_1968_1638.cif
_cod_data_source_block           Al2Ba1O4
_cod_original_cell_volume        207.0536
_cod_original_formula_sum        'Al2 Ba1 O4'
_cod_database_code               1527925
Crystal structure determination for Ge3 Bi2 Te6
Petrov, I.I.; Imamov, R.M.; Kristallografiya 15 (1970) 168–170; doi:

data_1527926
_publ_section_title
;
 Crystal structure determination for Ge3 Bi2 Te6
;
_journal_name_full               Kristallografiya
_journal_page_first              168
_journal_page_last               170
_journal_volume                  15
_journal_year                    1970
_chemical_formula_sum            'Bi2 Ge3 Te6'
_chemical_name_systematic        'Ge3 Bi2 Te6'
_space_group_IT_number           160
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   4.21
_cell_length_b                   4.21
_cell_length_c                   61
_cell_volume                     936.321
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Petrov_KRISAJ_1970_1908.cif
_cod_data_source_block           Bi2Ge3Te6
_cod_original_cell_volume        936.3208
_cod_database_code               1527926
Die Kristallstruktur von Blei-Barysilit, Pb3Si2O7
Petter, W.; Harnik, A.B.; Keppler, U.; Zeitschrift fuer Kristallographie, Kristallgeometrie, Kristallphysik, Kristallchemie (-144,1977) 133 (1971) 445–458; doi:

data_8103667
_publ_section_title
;
 Die Kristallstruktur von Blei-Barysilit, Pb3Si2O7
;
_journal_name_full
;
Zeitschrift fuer Kristallographie, Kristallgeometrie, Kristallphysik, 
Kristallchemie (-144,1977)
;
_journal_page_first              445
_journal_page_last               458
_journal_volume                  133
_journal_year                    1971
_chemical_formula_sum            'O7 Pb3 Si2'
_chemical_name_systematic        'Pb3 Si2 O7'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            18
_cell_length_a                   10.1264
_cell_length_b                   10.1264
_cell_length_c                   38.678
_cell_volume                     3434.826
_citation_journal_id_ASTM        ZEKGAX
_cod_data_source_file            Petter_ZEKGAX_1971_1414.cif
_cod_data_source_block           O7Pb3Si2
_cod_original_cell_volume        3434.827
_cod_database_code               8103667
Influence of cobalt-vacancies and nickel substitution on the magnetic properties of Ti Co2 Sn Heusler-type compound
Pierre, J.; Skolozdra, R.V.; Stadnyk, Yu.V.; Journal of Magnetism and Magnetic Materials 128 (1993) 93–100; doi:

data_1527927
_publ_section_title
;
 Influence of cobalt-vacancies and nickel substitution on the magnetic
 properties of Ti Co2 Sn Heusler-type compound
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              93
_journal_page_last               100
_journal_volume                  128
_journal_year                    1993
_chemical_formula_sum            'Co2 Sn Ti'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.067
_cell_length_b                   6.067
_cell_length_c                   6.067
_cell_volume                     223.317
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            Pierre_JMMMDC_1993_367.cif
_cod_data_source_block           Co2Sn1Ti1
_cod_original_cell_volume        223.3171
_cod_original_formula_sum        'Co2 Sn1 Ti1'
_cod_database_code               1527927
From nonmagnetic semiconductor to itinerant ferromagnet in the Ti Ni Sn - Ti Co Sn series
Pierre, J.; Skolozdra, R.V.; Gorelenko, Yu.K.; Kouacou, M.; Journal of Magnetism and Magnetic Materials 134 (1994) 95–105; doi:

data_1527928
_publ_section_title
;
 From nonmagnetic semiconductor to itinerant ferromagnet in the Ti Ni Sn -
 Ti Co Sn series
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              95
_journal_page_last               105
_journal_volume                  134
_journal_year                    1994
_chemical_formula_sum            'Co Ni Sn2 Ti2'
_chemical_name_systematic        '(Co Ni) Sn2 Ti2'
_space_group_IT_number           216
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.975
_cell_length_b                   5.975
_cell_length_c                   5.975
_cell_volume                     213.311
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            Pierre_JMMMDC_1994_360.cif
_cod_data_source_block           Co1Ni1Sn2Ti2
_cod_original_cell_volume        213.3112
_cod_original_formula_sum        'Co1 Ni1 Sn2 Ti2'
_cod_database_code               1527928
From nonmagnetic semiconductor to itinerant ferromagnet in the Ti Ni sn - Ti Co Sn series
Pierre, J.; Skolozdra, R.V.; Gorelenko, Yu.K.; Kouacou, M.; Journal of Magnetism and Magnetic Materials 134 (1994) 95–105; doi:

data_1527929
_publ_section_title
;
 From nonmagnetic semiconductor to itinerant ferromagnet in the Ti Ni sn -
 Ti Co Sn series
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              95
_journal_page_last               105
_journal_volume                  134
_journal_year                    1994
_chemical_formula_sum            'Co Sn Ti'
_space_group_IT_number           216
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.997
_cell_length_b                   5.997
_cell_length_c                   5.997
_cell_volume                     215.676
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            Pierre_JMMMDC_1994_366.cif
_cod_data_source_block           Co1Sn1Ti1
_cod_original_cell_volume        215.6762
_cod_original_formula_sum        'Co1 Sn1 Ti1'
_cod_database_code               1527929
Structure of P, P(I), P(II), P(III) - Tetrakistricarbonylnickel-tetraphosphorus hexaoxide
Pierron, E.D.; Wheatley, P.J.; Riess, J.G.; Acta Crystallographica (1,1948-23,1967) 21 (1966) 288–289; doi:

data_2310463
_publ_section_title
;
 Structure of P, P(I), P(II), P(III) -
 Tetrakistricarbonylnickel-tetraphosphorus hexaoxide
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              288
_journal_page_last               289
_journal_volume                  21
_journal_year                    1966
_chemical_formula_sum            'C12 Ni4 O18 P4'
_chemical_name_systematic        'P4 O6 (Ni (C O)3)4'
_space_group_IT_number           215
_symmetry_space_group_name_Hall  'P -4 2 3'
_symmetry_space_group_name_H-M   'P -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   8.811
_cell_length_b                   8.811
_cell_length_c                   8.811
_cell_volume                     684.031
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Pierron_ACCRA9_1966_1078.cif
_cod_data_source_block           C12Ni4O18P4
_cod_original_cell_volume        684.0307
_cod_database_code               2310463
A cursory investigation of intermediate phases Zr1-x Tix M2 and Hf1-x Tix M2 (M= Mo or W) systems
Pietrokowsky, P.; Transactions of the American Institute of Mining, Metallurgical and Petroleum Engineers 200 (1954) 219–226; doi:

data_1527930
_publ_section_title
;
 A cursory investigation of intermediate phases Zr1-x Tix M2 and Hf1-x Tix
 M2 (M= Mo or W) systems
;
_journal_name_full
;
Transactions of the American Institute of Mining, Metallurgical and Petroleum 
Engineers
;
_journal_page_first              219
_journal_page_last               226
_journal_volume                  200
_journal_year                    1954
_chemical_formula_sum            'Ti Zn2'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            4
_cell_length_a                   5.064
_cell_length_b                   5.064
_cell_length_c                   8.21
_cell_volume                     182.331
_citation_journal_id_ASTM        TAIMAF
_cod_data_source_file            Pietrokowsky_TAIMAF_1954_139.cif
_cod_data_source_block           Ti1Zn2
_cod_original_cell_volume        182.3313
_cod_original_formula_sum        'Ti1 Zn2'
_cod_database_code               1527930
A cursory investigation of intermediate phases Zr1-x Tix M2 and Hf1-x Tix M2 (M= Mo or W) systems
Pietrokowsky, P.; Transactions of the American Institute of Mining, Metallurgical and Petroleum Engineers 200 (1954) 219–226; doi:

data_1527931
_publ_section_title
;
 A cursory investigation of intermediate phases Zr1-x Tix M2 and Hf1-x Tix
 M2 (M= Mo or W) systems
;
_journal_name_full
;
Transactions of the American Institute of Mining, Metallurgical and Petroleum 
Engineers
;
_journal_page_first              219
_journal_page_last               226
_journal_volume                  200
_journal_year                    1954
_chemical_formula_sum            'Ti Zn3'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.9322
_cell_length_b                   3.9322
_cell_length_c                   3.9322
_cell_volume                     60.800
_citation_journal_id_ASTM        TAIMAF
_cod_data_source_file            Pietrokowsky_TAIMAF_1954_140.cif
_cod_data_source_block           Ti1Zn3
_cod_original_cell_volume        60.80045
_cod_original_formula_sum        'Ti1 Zn3'
_cod_database_code               1527931
A constitution diagram for the alloy system titanium-tin
Pietrokowsky, P.; Frink, E.P.; Transactions of the American Society for Metals 49 (1957) 339–358; doi:

data_1527932
_publ_section_title
;
 A constitution diagram for the alloy system titanium-tin
;
_journal_name_full
'Transactions of the American Society for Metals'
_journal_page_first              339
_journal_page_last               358
_journal_volume                  49
_journal_year                    1957
_chemical_formula_sum            'Sn Ti2'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   4.653
_cell_length_b                   4.653
_cell_length_c                   5.7
_cell_volume                     106.874
_citation_journal_id_ASTM        TASEA7
_cod_data_source_file            Pietrokowsky_TASEA7_1957_66.cif
_cod_data_source_block           Sn1Ti2
_cod_original_cell_volume        106.8739
_cod_original_formula_sum        'Sn1 Ti2'
_cod_database_code               1527932